#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/21/4312147.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4312147
loop_
_publ_author_name
'Łukasz Dobrzycki'
'Ewa Bulska'
'Dorota Anna Pawlak'
'Zygmunt Frukacz'
'Krzysztof Woźniak'
_publ_section_title
;
 Structure of YAG Crystals Doped/Substituted with Erbium and Ytterbium
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              7656
_journal_page_last               7664
_journal_paper_doi               10.1021/ic049920z
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'Al5 O12 Y2.21 Yb0.8'
_chemical_formula_weight         660.51
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           230
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   11.9813(14)
_cell_length_b                   11.9813(14)
_cell_length_c                   11.9813(14)
_cell_measurement_temperature    293(2)
_cell_volume                     1719.9(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0833
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       2
_diffrn_reflns_number            461
_diffrn_reflns_theta_full        40.22
_diffrn_reflns_theta_max         40.22
_diffrn_reflns_theta_min         4.17
_exptl_absorpt_coefficient_mu    23.922
_exptl_crystal_density_diffrn    5.102
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2421
_refine_diff_density_max         1.095
_refine_diff_density_min         -1.029
_refine_diff_density_rms         0.167
_refine_ls_extinction_coef       0.00079(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.423
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     18
_refine_ls_number_reflns         461
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.423
_refine_ls_R_factor_all          0.0409
_refine_ls_R_factor_gt           0.0154
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0263
_refine_ls_wR_factor_ref         0.0289
_reflns_number_gt                275
_reflns_number_total             461
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic049920zsi20040119_085908_17.cif
_cod_data_source_block           yb25
_cod_original_formula_sum        'Al5 O12 Y2.21 Yb0.80'
_cod_database_code               4312147
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'z, x, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z, x'
'-y, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z, x+1/2'
'y+3/4, x+1/4, -z+1/4'
'-y+3/4, -x+3/4, -z+3/4'
'y+1/4, -x+1/4, z+3/4'
'-y+1/4, x+3/4, z+1/4'
'x+3/4, z+1/4, -y+1/4'
'-x+1/4, z+3/4, y+1/4'
'-x+3/4, -z+3/4, -y+3/4'
'x+1/4, -z+1/4, y+3/4'
'z+3/4, y+1/4, -x+1/4'
'z+1/4, -y+1/4, x+3/4'
'-z+1/4, y+3/4, x+1/4'
'-z+3/4, -y+3/4, -x+3/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-x+1/2, y+1, -z+1'
'x+1, -y+1, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1, -x+1, -y+1/2'
'-z+1, -x+1/2, y+1'
'-z+1/2, x+1, -y+1'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1, -x+1'
'y+1, -z+1, -x+1/2'
'-y+1, -z+1/2, x+1'
'y+5/4, x+3/4, -z+3/4'
'-y+5/4, -x+5/4, -z+5/4'
'y+3/4, -x+3/4, z+5/4'
'-y+3/4, x+5/4, z+3/4'
'x+5/4, z+3/4, -y+3/4'
'-x+3/4, z+5/4, y+3/4'
'-x+5/4, -z+5/4, -y+5/4'
'x+3/4, -z+3/4, y+5/4'
'z+5/4, y+3/4, -x+3/4'
'z+3/4, -y+3/4, x+5/4'
'-z+3/4, y+5/4, x+3/4'
'-z+5/4, -y+5/4, -x+5/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z'
'-z, -x, -y'
'-z-1/2, x-1/2, y'
'z-1/2, x, -y-1/2'
'z, -x-1/2, y-1/2'
'-y, -z, -x'
'y, -z-1/2, x-1/2'
'-y-1/2, z-1/2, x'
'y-1/2, z, -x-1/2'
'-y-3/4, -x-1/4, z-1/4'
'y-3/4, x-3/4, z-3/4'
'-y-1/4, x-1/4, -z-3/4'
'y-1/4, -x-3/4, -z-1/4'
'-x-3/4, -z-1/4, y-1/4'
'x-1/4, -z-3/4, -y-1/4'
'x-3/4, z-3/4, y-3/4'
'-x-1/4, z-1/4, -y-3/4'
'-z-3/4, -y-1/4, x-1/4'
'-z-1/4, y-1/4, -x-3/4'
'z-1/4, -y-3/4, -x-1/4'
'z-3/4, y-3/4, x-3/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'x+1/2, -y, z'
'-x, y, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z, x, y+1/2'
'z, x+1/2, -y'
'z+1/2, -x, y'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z, x'
'-y, z, x+1/2'
'y, z+1/2, -x'
'-y-1/4, -x+1/4, z+1/4'
'y-1/4, x-1/4, z-1/4'
'-y+1/4, x+1/4, -z-1/4'
'y+1/4, -x-1/4, -z+1/4'
'-x-1/4, -z+1/4, y+1/4'
'x+1/4, -z-1/4, -y+1/4'
'x-1/4, z-1/4, y-1/4'
'-x+1/4, z+1/4, -y-1/4'
'-z-1/4, -y+1/4, x+1/4'
'-z+1/4, y+1/4, -x-1/4'
'z+1/4, -y-1/4, -x+1/4'
'z-1/4, y-1/4, x-1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Yb1 Yb 0.1250 0.0000 0.2500 0.00522(8) Uani 0.26 4 d SP . .
Y1 Y 0.1250 0.0000 0.2500 0.00522(8) Uani 0.74 4 d SP . .
Al1 Al 0.0000 0.0000 0.0000 0.0018(2) Uani 1 6 d S . .
Al2 Al 0.3750 0.0000 0.2500 0.0012(2) Uani 1 4 d S . .
O1 O 0.27997(14) 0.10104(14) 0.19970(14) 0.0043(3) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Yb Yb -0.3850 5.5486 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Yb1 O1 72.13(8) 18_545 43_444 ?
O1 Yb1 O1 158.43(9) 18_545 . ?
O1 Yb1 O1 112.14(8) 43_444 . ?
O1 Yb1 O1 112.14(8) 18_545 28_445 ?
O1 Yb1 O1 158.43(9) 43_444 28_445 ?
O1 Yb1 O1 72.13(8) . 28_445 ?
O1 Yb1 O1 67.44(8) 18_545 16_545 ?
O1 Yb1 O1 125.04(4) 43_444 16_545 ?
O1 Yb1 O1 94.86(5) . 16_545 ?
O1 Yb1 O1 74.02(7) 28_445 16_545 ?
O1 Yb1 O1 74.02(7) 18_545 35_445 ?
O1 Yb1 O1 94.86(5) 43_444 35_445 ?
O1 Yb1 O1 125.04(4) . 35_445 ?
O1 Yb1 O1 67.44(8) 28_445 35_445 ?
O1 Yb1 O1 107.66(8) 16_545 35_445 ?
O1 Yb1 O1 94.86(5) 18_545 9 ?
O1 Yb1 O1 74.02(7) 43_444 9 ?
O1 Yb1 O1 67.44(8) . 9 ?
O1 Yb1 O1 125.04(4) 28_445 9 ?
O1 Yb1 O1 74.01(8) 16_545 9 ?
O1 Yb1 O1 166.46(8) 35_445 9 ?
O1 Yb1 O1 125.04(4) 18_545 38_444 ?
O1 Yb1 O1 67.44(8) 43_444 38_444 ?
O1 Yb1 O1 74.02(7) . 38_444 ?
O1 Yb1 O1 94.86(5) 28_445 38_444 ?
O1 Yb1 O1 166.46(8) 16_545 38_444 ?
O1 Yb1 O1 74.01(8) 35_445 38_444 ?
O1 Yb1 O1 107.66(8) 9 38_444 ?
O1 Yb1 Al2 143.93(4) 18_545 . ?
O1 Yb1 Al2 143.93(4) 43_444 . ?
O1 Yb1 Al2 36.07(4) . . ?
O1 Yb1 Al2 36.07(4) 28_445 . ?
O1 Yb1 Al2 83.23(4) 16_545 . ?
O1 Yb1 Al2 96.77(4) 35_445 . ?
O1 Yb1 Al2 96.77(4) 9 . ?
O1 Yb1 Al2 83.23(4) 38_444 . ?
O1 Yb1 Al2 36.07(4) 18_545 50_556 ?
O1 Yb1 Al2 36.07(4) 43_444 50_556 ?
O1 Yb1 Al2 143.93(4) . 50_556 ?
O1 Yb1 Al2 143.93(4) 28_445 50_556 ?
O1 Yb1 Al2 96.77(4) 16_545 50_556 ?
O1 Yb1 Al2 83.23(4) 35_445 50_556 ?
O1 Yb1 Al2 83.23(4) 9 50_556 ?
O1 Yb1 Al2 96.77(4) 38_444 50_556 ?
Al2 Yb1 Al2 180.0 . 50_556 ?
O1 Yb1 Al1 96.31(4) 18_545 . ?
O1 Yb1 Al1 33.60(4) 43_444 . ?
O1 Yb1 Al1 97.29(4) . . ?
O1 Yb1 Al1 126.60(4) 28_445 . ?
O1 Yb1 Al1 158.60(4) 16_545 . ?
O1 Yb1 Al1 79.37(4) 35_445 . ?
O1 Yb1 Al1 94.54(4) 9 . ?
O1 Yb1 Al1 34.34(4) 38_444 . ?
Al2 Yb1 Al1 116.6 . . ?
Al2 Yb1 Al1 63.4 50_556 . ?
O1 Yb1 Al1 126.60(4) 18_545 38_444 ?
O1 Yb1 Al1 97.29(4) 43_444 38_444 ?
O1 Yb1 Al1 33.60(4) . 38_444 ?
O1 Yb1 Al1 96.31(4) 28_445 38_444 ?
O1 Yb1 Al1 79.37(4) 16_545 38_444 ?
O1 Yb1 Al1 158.60(4) 35_445 38_444 ?
O1 Yb1 Al1 34.34(4) 9 38_444 ?
O1 Yb1 Al1 94.54(4) 38_444 38_444 ?
Al2 Yb1 Al1 63.4 . 38_444 ?
Al2 Yb1 Al1 116.6 50_556 38_444 ?
Al1 Yb1 Al1 101.5 . 38_444 ?
O1 Al1 O1 86.59(8) 96 91 ?
O1 Al1 O1 86.59(8) 96 86 ?
O1 Al1 O1 86.59(8) 91 86 ?
O1 Al1 O1 180.00(4) 96 48_444 ?
O1 Al1 O1 93.41(8) 91 48_444 ?
O1 Al1 O1 93.41(8) 86 48_444 ?
O1 Al1 O1 93.41(8) 96 43_444 ?
O1 Al1 O1 180.00(10) 91 43_444 ?
O1 Al1 O1 93.41(8) 86 43_444 ?
O1 Al1 O1 86.59(8) 48_444 43_444 ?
O1 Al1 O1 93.41(8) 96 38_444 ?
O1 Al1 O1 93.41(8) 91 38_444 ?
O1 Al1 O1 180.00(14) 86 38_444 ?
O1 Al1 O1 86.59(8) 48_444 38_444 ?
O1 Al1 O1 86.59(8) 43_444 38_444 ?
O1 Al1 Yb1 88.46(5) 96 . ?
O1 Al1 Yb1 138.48(5) 91 . ?
O1 Al1 Yb1 134.21(5) 86 . ?
O1 Al1 Yb1 91.54(5) 48_444 . ?
O1 Al1 Yb1 41.52(5) 43_444 . ?
O1 Al1 Yb1 45.79(5) 38_444 . ?
O1 Al1 Yb1 45.79(5) 96 53 ?
O1 Al1 Yb1 91.54(5) 91 53 ?
O1 Al1 Yb1 41.52(5) 86 53 ?
O1 Al1 Yb1 134.21(5) 48_444 53 ?
O1 Al1 Yb1 88.46(5) 43_444 53 ?
O1 Al1 Yb1 138.48(5) 38_444 53 ?
Yb1 Al1 Yb1 113.6 . 53 ?
O1 Al1 Yb1 138.48(5) 96 9 ?
O1 Al1 Yb1 134.21(5) 91 9 ?
O1 Al1 Yb1 88.46(5) 86 9 ?
O1 Al1 Yb1 41.52(5) 48_444 9 ?
O1 Al1 Yb1 45.79(5) 43_444 9 ?
O1 Al1 Yb1 91.54(5) 38_444 9 ?
Yb1 Al1 Yb1 66.4 . 9 ?
Yb1 Al1 Yb1 113.6 53 9 ?
O1 Al1 Yb1 41.52(5) 96 57 ?
O1 Al1 Yb1 45.79(5) 91 57 ?
O1 Al1 Yb1 91.54(5) 86 57 ?
O1 Al1 Yb1 138.48(5) 48_444 57 ?
O1 Al1 Yb1 134.21(5) 43_444 57 ?
O1 Al1 Yb1 88.46(5) 38_444 57 ?
Yb1 Al1 Yb1 113.6 . 57 ?
Yb1 Al1 Yb1 66.4 53 57 ?
Yb1 Al1 Yb1 180.0 9 57 ?
O1 Al1 Y1 91.54(5) 96 49 ?
O1 Al1 Y1 41.52(5) 91 49 ?
O1 Al1 Y1 45.79(5) 86 49 ?
O1 Al1 Y1 88.46(5) 48_444 49 ?
O1 Al1 Y1 138.48(5) 43_444 49 ?
O1 Al1 Y1 134.21(5) 38_444 49 ?
Yb1 Al1 Y1 180.0 . 49 ?
Yb1 Al1 Y1 66.4 53 49 ?
Yb1 Al1 Y1 113.6 9 49 ?
Yb1 Al1 Y1 66.4 57 49 ?
O1 Al1 Y1 134.21(5) 96 5 ?
O1 Al1 Y1 88.46(5) 91 5 ?
O1 Al1 Y1 138.48(5) 86 5 ?
O1 Al1 Y1 45.79(5) 48_444 5 ?
O1 Al1 Y1 91.54(5) 43_444 5 ?
O1 Al1 Y1 41.52(5) 38_444 5 ?
Yb1 Al1 Y1 66.4 . 5 ?
Yb1 Al1 Y1 180.0 53 5 ?
Yb1 Al1 Y1 66.4 9 5 ?
Yb1 Al1 Y1 113.6 57 5 ?
Y1 Al1 Y1 113.6 49 5 ?
O1 Al1 Y1 45.79(5) 96 53 ?
O1 Al1 Y1 91.54(5) 91 53 ?
O1 Al1 Y1 41.52(5) 86 53 ?
O1 Al1 Y1 134.21(5) 48_444 53 ?
O1 Al1 Y1 88.46(5) 43_444 53 ?
O1 Al1 Y1 138.48(5) 38_444 53 ?
Yb1 Al1 Y1 113.6 . 53 ?
Yb1 Al1 Y1 0.0 53 53 ?
Yb1 Al1 Y1 113.6 9 53 ?
Yb1 Al1 Y1 66.4 57 53 ?
Y1 Al1 Y1 66.4 49 53 ?
Y1 Al1 Y1 180.0 5 53 ?
O1 Al1 Y1 138.48(5) 96 9 ?
O1 Al1 Y1 134.21(5) 91 9 ?
O1 Al1 Y1 88.46(5) 86 9 ?
O1 Al1 Y1 41.52(5) 48_444 9 ?
O1 Al1 Y1 45.79(5) 43_444 9 ?
O1 Al1 Y1 91.54(5) 38_444 9 ?
Yb1 Al1 Y1 66.4 . 9 ?
Yb1 Al1 Y1 113.6 53 9 ?
Yb1 Al1 Y1 0.0 9 9 ?
Yb1 Al1 Y1 180.0 57 9 ?
Y1 Al1 Y1 113.6 49 9 ?
Y1 Al1 Y1 66.4 5 9 ?
Y1 Al1 Y1 113.6 53 9 ?
O1 Al1 Y1 41.52(5) 96 57 ?
O1 Al1 Y1 45.79(5) 91 57 ?
O1 Al1 Y1 91.54(5) 86 57 ?
O1 Al1 Y1 138.48(5) 48_444 57 ?
O1 Al1 Y1 134.21(5) 43_444 57 ?
O1 Al1 Y1 88.46(5) 38_444 57 ?
Yb1 Al1 Y1 113.6 . 57 ?
Yb1 Al1 Y1 66.4 53 57 ?
Yb1 Al1 Y1 180.0 9 57 ?
Yb1 Al1 Y1 0.0 57 57 ?
Y1 Al1 Y1 66.4 49 57 ?
Y1 Al1 Y1 113.6 5 57 ?
Y1 Al1 Y1 66.4 53 57 ?
Y1 Al1 Y1 180.0 9 57 ?
O1 Al1 Yb1 134.21(5) 96 5 ?
O1 Al1 Yb1 88.46(5) 91 5 ?
O1 Al1 Yb1 138.48(5) 86 5 ?
O1 Al1 Yb1 45.79(5) 48_444 5 ?
O1 Al1 Yb1 91.54(5) 43_444 5 ?
O1 Al1 Yb1 41.52(5) 38_444 5 ?
Yb1 Al1 Yb1 66.4 . 5 ?
Yb1 Al1 Yb1 180.0 53 5 ?
Yb1 Al1 Yb1 66.4 9 5 ?
Yb1 Al1 Yb1 113.6 57 5 ?
Y1 Al1 Yb1 113.6 49 5 ?
Y1 Al1 Yb1 0.0 5 5 ?
Y1 Al1 Yb1 180.0 53 5 ?
Y1 Al1 Yb1 66.4 9 5 ?
Y1 Al1 Yb1 113.6 57 5 ?
O1 Al1 Yb1 91.54(5) 96 49 ?
O1 Al1 Yb1 41.52(5) 91 49 ?
O1 Al1 Yb1 45.79(5) 86 49 ?
O1 Al1 Yb1 88.46(5) 48_444 49 ?
O1 Al1 Yb1 138.48(5) 43_444 49 ?
O1 Al1 Yb1 134.21(5) 38_444 49 ?
Yb1 Al1 Yb1 180.0 . 49 ?
Yb1 Al1 Yb1 66.4 53 49 ?
Yb1 Al1 Yb1 113.6 9 49 ?
Yb1 Al1 Yb1 66.4 57 49 ?
Y1 Al1 Yb1 0.0 49 49 ?
Y1 Al1 Yb1 113.6 5 49 ?
Y1 Al1 Yb1 66.4 53 49 ?
Y1 Al1 Yb1 113.6 9 49 ?
Y1 Al1 Yb1 66.4 57 49 ?
Yb1 Al1 Yb1 113.6 5 49 ?
O1 Al1 O1 113.80(6) 96 . ?
O1 Al1 O1 117.44(6) 91 . ?
O1 Al1 O1 148.13(5) 86 . ?
O1 Al1 O1 66.20(6) 48_444 . ?
O1 Al1 O1 62.56(6) 43_444 . ?
O1 Al1 O1 31.87(5) 38_444 . ?
Yb1 Al1 O1 32.04(2) . . ?
Yb1 Al1 O1 145.56(2) 53 . ?
Yb1 Al1 O1 59.91(2) 9 . ?
Yb1 Al1 O1 120.09(2) 57 . ?
Y1 Al1 O1 147.96(2) 49 . ?
Y1 Al1 O1 34.44(2) 5 . ?
Y1 Al1 O1 145.56(2) 53 . ?
Y1 Al1 O1 59.91(2) 9 . ?
Y1 Al1 O1 120.09(2) 57 . ?
Yb1 Al1 O1 34.44(2) 5 . ?
Yb1 Al1 O1 147.96(2) 49 . ?
O1 Al1 Al1 127.64(5) 96 49_666 ?
O1 Al1 Al1 127.64(5) 91 49_666 ?
O1 Al1 Al1 127.64(5) 86 49_666 ?
O1 Al1 Al1 52.36(5) 48_444 49_666 ?
O1 Al1 Al1 52.36(5) 43_444 49_666 ?
O1 Al1 Al1 52.36(5) 38_444 49_666 ?
Yb1 Al1 Al1 39.2 . 49_666 ?
Yb1 Al1 Al1 140.8 53 49_666 ?
Yb1 Al1 Al1 39.2 9 49_666 ?
Yb1 Al1 Al1 140.8 57 49_666 ?
Y1 Al1 Al1 140.8 49 49_666 ?
Y1 Al1 Al1 39.2 5 49_666 ?
Y1 Al1 Al1 140.8 53 49_666 ?
Y1 Al1 Al1 39.2 9 49_666 ?
Y1 Al1 Al1 140.8 57 49_666 ?
Yb1 Al1 Al1 39.2 5 49_666 ?
Yb1 Al1 Al1 140.8 49 49_666 ?
O1 Al1 Al1 20.71(2) . 49_666 ?
O1 Al2 O1 114.51(6) 89_655 28_445 ?
O1 Al2 O1 99.80(11) 89_655 68_656 ?
O1 Al2 O1 114.51(6) 28_445 68_656 ?
O1 Al2 O1 114.51(6) 89_655 . ?
O1 Al2 O1 99.80(11) 28_445 . ?
O1 Al2 O1 114.51(6) 68_656 . ?
O1 Al2 Yb1 130.10(6) 89_655 . ?
O1 Al2 Yb1 49.90(6) 28_445 . ?
O1 Al2 Yb1 130.10(6) 68_656 . ?
O1 Al2 Yb1 49.90(6) . . ?
O1 Al2 Y1 49.90(6) 89_655 50_656 ?
O1 Al2 Y1 130.10(6) 28_445 50_656 ?
O1 Al2 Y1 49.90(6) 68_656 50_656 ?
O1 Al2 Y1 130.10(6) . 50_656 ?
Yb1 Al2 Y1 180.0 . 50_656 ?
O1 Al2 Yb1 49.90(6) 89_655 50_656 ?
O1 Al2 Yb1 130.10(6) 28_445 50_656 ?
O1 Al2 Yb1 49.90(6) 68_656 50_656 ?
O1 Al2 Yb1 130.10(6) . 50_656 ?
Yb1 Al2 Yb1 180.0 . 50_656 ?
Y1 Al2 Yb1 0.0 50_656 50_656 ?
O1 Al2 O1 144.65(5) 89_655 54_655 ?
O1 Al2 O1 57.58(8) 28_445 54_655 ?
O1 Al2 O1 62.16(8) 68_656 54_655 ?
O1 Al2 O1 100.81(5) . 54_655 ?
Yb1 Al2 O1 74.30(3) . 54_655 ?
Y1 Al2 O1 105.70(3) 50_656 54_655 ?
Yb1 Al2 O1 105.70(3) 50_656 54_655 ?
O1 Al2 O1 57.58(8) 89_655 45_445 ?
O1 Al2 O1 62.16(8) 28_445 45_445 ?
O1 Al2 O1 100.81(5) 68_656 45_445 ?
O1 Al2 O1 144.65(5) . 45_445 ?
Yb1 Al2 O1 105.70(3) . 45_445 ?
Y1 Al2 O1 74.30(3) 50_656 45_445 ?
Yb1 Al2 O1 74.30(3) 50_656 45_445 ?
O1 Al2 O1 94.200(16) 54_655 45_445 ?
O1 Al2 O1 62.16(8) 89_655 77 ?
O1 Al2 O1 100.81(5) 28_445 77 ?
O1 Al2 O1 144.65(5) 68_656 77 ?
O1 Al2 O1 57.58(8) . 77 ?
Yb1 Al2 O1 74.30(3) . 77 ?
Y1 Al2 O1 105.70(3) 50_656 77 ?
Yb1 Al2 O1 105.70(3) 50_656 77 ?
O1 Al2 O1 148.60(6) 54_655 77 ?
O1 Al2 O1 94.200(16) 45_445 77 ?
O1 Al2 O1 100.81(5) 89_655 22_554 ?
O1 Al2 O1 144.65(5) 28_445 22_554 ?
O1 Al2 O1 57.58(8) 68_656 22_554 ?
O1 Al2 O1 62.16(8) . 22_554 ?
Yb1 Al2 O1 105.70(3) . 22_554 ?
Y1 Al2 O1 74.30(3) 50_656 22_554 ?
Yb1 Al2 O1 74.30(3) 50_656 22_554 ?
O1 Al2 O1 94.200(16) 54_655 22_554 ?
O1 Al2 O1 148.60(6) 45_445 22_554 ?
O1 Al2 O1 94.200(16) 77 22_554 ?
Al2 O1 Al1 130.60(10) . 38_444 ?
Al2 O1 Yb1 94.03(7) . . ?
Al1 O1 Yb1 104.87(7) 38_444 . ?
Al2 O1 Y1 120.69(8) . 5 ?
Al1 O1 Y1 99.87(7) 38_444 5 ?
Yb1 O1 Y1 101.58(7) . 5 ?
Al2 O1 Yb1 120.69(8) . 5 ?
Al1 O1 Yb1 99.87(7) 38_444 5 ?
Yb1 O1 Yb1 101.58(7) . 5 ?
Y1 O1 Yb1 0.0 5 5 ?
Al2 O1 O1 135.08(12) . 9 ?
Al1 O1 O1 46.70(4) 38_444 9 ?
Yb1 O1 O1 58.81(6) . 9 ?
Y1 O1 O1 100.72(5) 5 9 ?
Yb1 O1 O1 100.72(5) 5 9 ?
Al2 O1 O1 161.24(10) . 5 ?
Al1 O1 O1 46.70(4) 38_444 5 ?
Yb1 O1 O1 104.59(5) . 5 ?
Y1 O1 O1 53.75(6) 5 5 ?
Yb1 O1 O1 53.75(6) 5 5 ?
O1 O1 O1 60.0 9 5 ?
Al2 O1 O1 40.10(6) . 28_445 ?
Al1 O1 O1 133.87(11) 38_444 28_445 ?
Yb1 O1 O1 53.93(4) . 28_445 ?
Y1 O1 O1 122.90(10) 5 28_445 ?
Yb1 O1 O1 122.90(10) 5 28_445 ?
O1 O1 O1 103.85(9) 9 28_445 ?
O1 O1 O1 158.43(4) 5 28_445 ?
Al2 O1 O1 103.12(9) . 81 ?
Al1 O1 O1 43.30(4) 38_444 81 ?
Yb1 O1 O1 147.22(6) . 81 ?
Y1 O1 O1 93.45(5) 5 81 ?
Yb1 O1 O1 93.45(5) 5 81 ?
O1 O1 O1 90.0 9 81 ?
O1 O1 O1 61.89(4) 5 81 ?
O1 O1 O1 136.61(8) 28_445 81 ?
Al2 O1 O1 90.11(9) . 77 ?
Al1 O1 O1 43.30(4) 38_444 77 ?
Yb1 O1 O1 96.62(5) . 77 ?
Y1 O1 O1 142.43(6) 5 77 ?
Yb1 O1 O1 142.43(6) 5 77 ?
O1 O1 O1 61.89(4) 9 77 ?
O1 O1 O1 90.0 5 77 ?
O1 O1 O1 94.36(9) 28_445 77 ?
O1 O1 O1 56.21(8) 81 77 ?
Al2 O1 O1 101.05(6) . 38_444 ?
Al1 O1 O1 127.34(5) 38_444 38_444 ?
Yb1 O1 O1 55.23(6) . 38_444 ?
Y1 O1 O1 50.75(5) 5 38_444 ?
Yb1 O1 O1 50.75(5) 5 38_444 ?
O1 O1 O1 91.62(3) 9 38_444 ?
O1 O1 O1 88.01(4) 5 38_444 ?
O1 O1 O1 77.70(6) 28_445 38_444 ?
O1 O1 O1 143.78(8) 81 38_444 ?
O1 O1 O1 150.01(7) 77 38_444 ?
Al2 O1 O1 85.63(7) . 22_554 ?
Al1 O1 O1 99.53(9) 38_444 22_554 ?
Yb1 O1 O1 147.74(8) . 22_554 ?
Y1 O1 O1 53.00(4) 5 22_554 ?
Yb1 O1 O1 53.00(4) 5 22_554 ?
O1 O1 O1 136.95(9) 9 22_554 ?
O1 O1 O1 77.43(9) 5 22_554 ?
O1 O1 O1 118.97(9) 28_445 22_554 ?
O1 O1 O1 62.54(7) 81 22_554 ?
O1 O1 O1 115.63(7) 77 22_554 ?
O1 O1 O1 93.11(6) 38_444 22_554 ?
Al2 O1 O1 32.74(3) . 89_655 ?
Al1 O1 O1 98.16(9) 38_444 89_655 ?
Yb1 O1 O1 110.57(6) . 89_655 ?
Y1 O1 O1 137.37(9) 5 89_655 ?
Yb1 O1 O1 137.37(9) 5 89_655 ?
O1 O1 O1 119.54(9) 9 89_655 ?
O1 O1 O1 136.11(5) 5 89_655 ?
O1 O1 O1 62.95(3) 28_445 89_655 ?
O1 O1 O1 74.36(9) 81 89_655 ?
O1 O1 O1 61.06(8) 77 89_655 ?
O1 O1 O1 133.77(4) 38_444 89_655 ?
O1 O1 O1 86.09(5) 22_554 89_655 ?
Al2 O1 O1 32.74(3) . 68_656 ?
Al1 O1 O1 140.81(10) 38_444 68_656 ?
Yb1 O1 O1 110.57(6) . 68_656 ?
Y1 O1 O1 89.08(7) 5 68_656 ?
Yb1 O1 O1 89.08(7) 5 68_656 ?
O1 O1 O1 166.64(11) 9 68_656 ?
O1 O1 O1 133.24(11) 5 68_656 ?
O1 O1 O1 62.95(3) 28_445 68_656 ?
O1 O1 O1 98.52(9) 81 68_656 ?
O1 O1 O1 114.80(8) 77 68_656 ?
O1 O1 O1 87.57(5) 38_444 68_656 ?
O1 O1 O1 56.40(8) 22_554 68_656 ?
O1 O1 O1 54.10(7) 89_655 68_656 ?
Al2 O1 Al2 87.04(6) . 81 ?
Al1 O1 Al2 74.46(5) 38_444 81 ?
Yb1 O1 Al2 178.92(7) . 81 ?
Y1 O1 Al2 77.77(4) 5 81 ?
Yb1 O1 Al2 77.77(4) 5 81 ?
O1 O1 Al2 120.41(5) 9 81 ?
O1 O1 Al2 74.33(6) 5 81 ?
O1 O1 Al2 127.14(3) 28_445 81 ?
O1 O1 Al2 32.31(4) 81 81 ?
O1 O1 Al2 83.47(7) 77 81 ?
O1 O1 Al2 124.47(9) 38_444 81 ?
O1 O1 Al2 32.21(4) 22_554 81 ?
O1 O1 Al2 70.42(7) 89_655 81 ?
O1 O1 Al2 70.32(6) 68_656 81 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Yb1 O1 2.2969(17) 18_545 ?
Yb1 O1 2.2969(17) 43_444 ?
Yb1 O1 2.2969(17) . ?
Yb1 O1 2.2969(17) 28_445 ?
Yb1 O1 2.4364(18) 16_545 ?
Yb1 O1 2.4364(18) 35_445 ?
Yb1 O1 2.4364(18) 9 ?
Yb1 O1 2.4364(18) 38_444 ?
Yb1 Al2 2.9953(4) . ?
Yb1 Al2 2.9953(4) 50_556 ?
Yb1 Al1 3.3489(4) . ?
Yb1 Al1 3.3489(4) 38_444 ?
Al1 O1 1.9177(17) 96 ?
Al1 O1 1.9177(17) 91 ?
Al1 O1 1.9177(17) 86 ?
Al1 O1 1.9177(17) 48_444 ?
Al1 O1 1.9177(17) 43_444 ?
Al1 O1 1.9177(17) 38_444 ?
Al1 Yb1 3.3489(4) 53 ?
Al1 Yb1 3.3489(4) 9 ?
Al1 Yb1 3.3489(4) 57 ?
Al1 Y1 3.3489(4) 49 ?
Al1 Y1 3.3489(4) 5 ?
Al1 Y1 3.3489(4) 53 ?
Al1 Y1 3.3489(4) 9 ?
Al1 Y1 3.3489(4) 57 ?
Al1 Yb1 3.3489(4) 5 ?
Al1 Yb1 3.3489(4) 49 ?
Al1 O1 4.2944(19) . ?
Al1 Al1 20.752(2) 49_666 ?
Al2 O1 1.7678(16) 89_655 ?
Al2 O1 1.7678(16) 28_445 ?
Al2 O1 1.7678(16) 68_656 ?
Al2 O1 1.7678(16) . ?
Al2 Y1 2.9953(4) 50_656 ?
Al2 Yb1 2.9953(4) 50_656 ?
Al2 O1 3.3071(18) 54_655 ?
Al2 O1 3.3070(18) 45_445 ?
Al2 O1 3.3070(18) 77 ?
Al2 O1 3.3070(18) 22_554 ?
O1 Al1 1.9177(17) 38_444 ?
O1 Y1 2.4364(18) 5 ?
O1 Yb1 2.4364(18) 5 ?
O1 O1 2.630(3) 9 ?
O1 O1 2.630(3) 5 ?
O1 O1 2.705(3) 28_445 ?
O1 O1 2.791(3) 81 ?
O1 O1 2.791(3) 77 ?
O1 O1 2.851(4) 38_444 ?
O1 O1 2.933(3) 22_554 ?
O1 O1 2.974(3) 89_655 ?
O1 O1 2.974(3) 68_656 ?
O1 Al2 3.3070(18) 81 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Al1 Al1 Al1 O1 3.40(6) ? . 49_666 43_444 ?
